Research Article  Open Access
ChienLung Huang, YuJia Gao, TaoLiang Chuang, Vincent K. S. Hsiao, TairI Wu, "Study of the Behavior of Titanium Alloys as the Cathode for Photovoltaic Hydrogen Production", International Journal of Photoenergy, vol. 2013, Article ID 857491, 6 pages, 2013. https://doi.org/10.1155/2013/857491
Study of the Behavior of Titanium Alloys as the Cathode for Photovoltaic Hydrogen Production
Abstract
CPTi and Ti153 were adopted in this study to observe their electrochemical behavior in serving as the cathode for photovoltaic hydrogen production. The designed cyclic hydrogenationsolution heat treating processes were performed to increase the hydrogen uptake for both alloys. The results are as follows. (1) Both arsenic trioxide and thiourea showed hydrogenation promotive effect on CPTi, while thiourea was an inhibitor for Ti153 under the applied conditions. (2) Arsenic trioxide showed hydrogenation promotive effect on both Ti153 and CPTi in this study. (3) Ti153 demonstrated superiority to CPTi when serves as the cathode for photovoltaic hydrogen production. The hydrogen mass payload for Ti153 is 68 times larger than that for CPTi.
1. Introduction
The available renewable energy on the earth’s surface includes the solar power, the wind power, and the hydroelectric power which uses the fall of the river, tidal power, or ocean current power. The wind power and hydroelectric power are, however, significantly limited by the location on the earth, the terrain, or the climate. The solar energy has less restriction in contrast to the abovementioned power sources [1–5]. The applications of sunlight can be divided into two parts: solar thermal energy and photovoltaic (PV). The application of the former is to transform solar energy to obtain heat which could be used in air condition, offer the hot water, or run a heat engine to make electricity [6–8]. PV energy systems employ solar panels in directly converting the sunlight into electricity [9, 10].
Since the solar power and the wind power are intermittent energy which means it is interruptible and cannot be a stable source due to the variation of the illuminance of sunlight and the change of wind field, for the commercial feasibility considerations, people have to store the energy when they can give. Unlike other forms of energy, electricity must be utilized when it is being generated or converted immediately into another form of energy. The PV energy system is usually equipped with an electrolyzer and a hydrogen storage tank (see Figure 1) [1, 2, 11, 12]. Although the gaseous hydrogen is convenient to store, transport, and apply, the inherent low volume payload rate and high flammability are the death wounds [13, 14]. It is safer to store hydrogen in solid state, but the increase of hydrogen mass payload rate is still technological challenge [15].
Electrolysis of aqueous sulfuric acid results in hydrogen at cathode surface. The resulted hydrogen can be driven into the cathode as solid solutes or hydrides by adequately adding hydrogenation promoters and selecting cathode material [16–20]. Ti15V3Al3Cr3Sn alloy (Ti153), as a commonly used βTi alloy, was chosen in this study to compare with commercial purity titanium (CPTi) to see the influences of the chemical additives and cathode material on the electrolytic hydrogen uptake.
2. Materials and Methods
The cathode materials in sheet form were received at rolled and process annealed state. The specimens were sheared from the received sheets to be 40 × 14 × 1 mm^{3} for CPTi, while they are 62 × 16 × 0.4 mm^{3} for Ti153, vacuum annealed at 1000°C for 30 minutes and furnace cooled to room temperature. The vacuum annealed specimens were abraded with emery paper (up to grit 1200) and further lapped to minimize the interference of surface oxides on hydrogenation. Table 1 listed the chemical compositions of the asreceived sheets. Table 2 summarized the surface roughness measured by employing a profile measuring system (Dektek 150, Veeco).
(a)  
 
(b)  

 
: The arithmetic mean of the departure of the profile from the mean line. : The rootmeansquare parameter corresponding to . 
The processing parameters listed in Table 3 were designed to reveal the effect of the additives on the electrochemical behavior of cathode and grouped into three sets according to the additives in the electrolyte as follows: no additive in 1 N H_{2}SO_{4(aq)}, denoted by S, 1 N H_{2}SO_{4(aq)} by adding 0.005 M arsenic trioxide (As_{2}O_{3}), denoted by A, (3) 1 N H_{2}SO_{4(aq)} by adding 0.01 M thiourea (SC(NH_{2})_{2}), denoted by T, respectively. Electrolytic hydrogenation was performed at 5 mA/cm^{2} for 15 h in various electrolytes, respectively. The preheat treatment was schematically shown in Figure 2(a). Figure 2(b) showed the schematic diagram of cyclic hydrogenationsolution heat treating processes. Electrolytic hydrogenation of the cyclic process was performed in 1 N H_{2}SO_{4(aq)} containing As_{2}O_{3} (0.1 g/L) at 50 mA/cm^{2} for 30 h on CPTi specimens while for 10 h on Ti153 ones preventing the hydride layer from spallation or the specimen from cracking. The subsequent solution treatments were accomplished in a muffle furnace at 300°C for 2 h. Table 4 listed designations and processing parameters of the cyclic hydrogenationsolution processes.


(a)
(b)
The effects of processing parameters on the hydrogenation behavior were evaluated qualitatively by utilizing Xray diffractometry (XRD: X’Pert PRO MPD, PANalytical, the Netherlands, 45 kV40 mA) and  curve monitoring. The quantitative cathodic behavior and hydrogen uptake of CPTi and Ti153 specimens were analyzed by the employment of glow discharge optical spectrometry (GDOS: LECO GDS750).
3. Results and Discussion
Large amounts of hydrogen absorption would lead to the shift and broadening of α peaks and presence of δ peaks in the XRD patterns of CPTi specimens. Patterns S, T, and A in Figure 3(a) exhibited δ peaks in contrast to pattern O [17–20]. The lower diffraction angle of the δ (220) peak implies higher hydrogen content for the certain adopted process. Both values of the relative peak height ratio, δ (200)/α (101), and the angular position of δ (220) peak for S, T, and A processes qualitatively corroborated stronger hydrogenation promotive effect of arsenic trioxide than that of thiourea on CPTi specimens. The cathodic potentials in Figure 4(a) were A, T, and S in an ascending order, which means that both arsenic trioxide and thiourea are hydrogenation promoters during cathodic charging [19–22]. Figure 3(b) showed the XRD patterns for Ti153 specimens after S, T and A treatments. Electrolytic hydrogenation under the applied conditions did not lead to precipitation of hydrides but to a shift of β peaks. The larger angle the peak shifted, the larger amount of hydrogen the specimen absorbed [23]. The angular shifts of all four β peaks in Figure 3(b) were A, S and T in a descending order, while the cathodic potentials in Figure 4(b) were A, S, and T in an ascending order. The higher cathodic potentials and lower hydrogen absorption for process T performed on Ti153 specimens mean that thiourea in 1N H_{2}SO_{4(aq)} is a hydrogenation inhibitor for Ti153 specimens under the conditions. Since arsenic trioxide was a hydrogen promoter for both CPTi and Ti153 specimens during cathodic charging, it was chosen as the hydriding catalyst added in the following cyclic hydrogenationsolution heat treating processes to enhance hydrogen uptake.
(a)
(b)
(a)
(b)
Figure 5 showed the hydrogen depth profiles of OCH3 and OBI3 specimens after cyclic hydrogenationsolution treatment. Quantitative hydrogen distribution curves were obtained by employing GDOS. The analyses of hydrogen uptake were accomplished by simply summing the specific hydrogen content (SHC) from the specimen surface to the maximum hydrogen diffusion depth (MHD) listed in Table 5. The SHC can be derived from total hydrogen content (THC) as shown in the following formula [24, 25]:

where and are the depth of layer and layer , respectively, is the local hydrogen content in weight or atomic percentage, is the differential quantity of local mass, is the local density, is the differential quantity of local volume, is the crosssectional area concerned, andis the differential quantity along the depth. Since is constant, the formula in (1) can be further simplified as:
Since the area in (2) is a determined value, the comparison of SHC is equivalent to that of THC. SHC values can outcome automatically after GDOS analyses. The SHC values were adopted to list in Table 5 to see the hydrogen mass payload between CPTi and Ti153 cathodes. The SHC_{0MHD} for OCH3 and OBI3 are 38.2 mg/m^{2} and 860 mg/m^{2}, respectively. The charging period for OCH3 was three times longer than that for OBI3. The ratio of hydrogen absorption for OBI3 to that for OCH3 can be easily estimated as (860 × 3) ÷ 38.2 = 67.5. The specific weight of Ti153 is about 4.42 while that of CPTi is about 4.51. Higher hydrogen uptake ability combines lower density. Ti153 shows obvious superiority to CPTi in hydrogen mass payload.
4. Conclusions
Both arsenic trioxide and thiourea are hydrogenation promoters for CPTi, while thiourea shows inhibitive effect on Ti153 under the applied conditions. Arsenic trioxide is a hydrogenation promoter for both Ti153 and CPTi in this study. Ti153 is superior to CPTi in serving as the cathode for photovoltaic hydrogen production. The hydrogen mass payload for Ti153 is estimated to be more than 68 times in contrast to that for CPTi.
Acknowledgments
The authors are grateful for the financial support of this research by the Tatung University and the National Science Council under Grant nos. B101T08012 and NSC 1012622E036002CC3, respectively.
References
 S. Iu. Bortnikov, N. S. Lidorenko, G. F. Muchnik, S. V. Riabikov, and D. S. Strebkov, SolarEnergy Perspectives, International Energy Agency, 2011.
 P. Gipe, “The wind industry's experience with aesthetic criticism,” Leonardo, vol. 26, no. 3, pp. 243–248, 1993. View at: Google Scholar
 Association for Industrial Archaeology, Industrial Archaeology Review, vol. 1011, Oxford University Press, 1987.
 D. Kerr, “Marine energy,” Philosophical Transactions of the Royal Society A, vol. 365, no. 1853, pp. 971–992, 2007. View at: Publisher Site  Google Scholar
 F. Qiang, “Radiation (solar),” in Encyclopedia of Atmospheric Sciences, J. R. Holton, Ed., pp. 1859–1863, Academic Press, 2003. View at: Google Scholar
 B. Sorensen, Renewable Energy: Physics, Engineering, Environmental Impacts, Economics & Planning, Elsevier Science, 2010.
 B. M. Diaconu, “Energy analysis of a solarassisted ejector cycle air conditioning system with low temperature thermal energy storage,” Renewable Energy, vol. 37, no. 1, pp. 266–276, 2012. View at: Publisher Site  Google Scholar
 Y. Tian and C. Y. Zhao, “A review of solar collectors and thermal energy storage in solar thermal applications,” Applied Energy, vol. 104, pp. 538–553, 2013. View at: Google Scholar
 L. Li, L. Duan, Y. Xu, M. Gorlov, A. Hagfeldt, and L. Sun, “A photoelectrochemical device for visible light driven water splitting by a molecular ruthenium catalyst assembled on dyesensitized nanostructured TiO_{2},” Chemical Communications, vol. 46, no. 39, pp. 7307–7309, 2010. View at: Publisher Site  Google Scholar
 T. L. Gibson and N. A. Kelly, “Predicting efficiency of solar powered hydrogen generation using photovoltaicelectrolysis devices,” International Journal of Hydrogen Energy, vol. 35, no. 3, pp. 900–911, 2010. View at: Publisher Site  Google Scholar
 J. M. Pearce, “Photovoltaics—a path to sustainable futures,” Futures, vol. 34, no. 7, pp. 663–674, 2002. View at: Publisher Site  Google Scholar
 J. L. BernalAgustín and R. DufoLópez, “Hourly energy management for gridconnected windhydrogen systems,” International Journal of Hydrogen Energy, vol. 33, no. 22, pp. 6401–6413, 2008. View at: Publisher Site  Google Scholar
 R. B. Gupta, Hydrogen Fuel: Production, Transport, and Storage, Taylor & Francis, 2009.
 F. Rigas and P. Amyotte, Hydrogen Safety, CRC Press, 2012.
 J. O. Jensen, A. P. Vestbø, Q. Li, and N. J. Bjerrum, “The energy efficiency of onboard hydrogen storage,” Journal of Alloys and Compounds, vol. 446447, pp. 723–728, 2007. View at: Publisher Site  Google Scholar
 J. F. Newman and L. L. Shreir, “Role of hydrides in hydrogen entry into steel from solutions containing promoters,” Corrosion Science, vol. 9, no. 8, pp. 631–641, 1969. View at: Google Scholar
 T.I. Wu, C.T. Liu, and J.K. Wu, “Use of thiourea to inhibit the incorporation of hydrogen in Ti and Ti6Al4V alloy,” Materials Letters, vol. 30, no. 56, pp. 377–383, 1997. View at: Google Scholar
 T.I. Wu and J.K. Wu, “Effects of thiourea and its derivatives on the electrolytic hydrogenation behavior of Ti6Al4V alloy,” Materials Letters, vol. 53, no. 3, pp. 193–199, 2002. View at: Publisher Site  Google Scholar
 T.I. Wu and J.K. Wu, “Effects of electrolytic hydrogenating parameters on structure and composition of surface hydrides of CPTi and Ti6Al4V alloy,” Materials Chemistry and Physics, vol. 74, no. 1, pp. 5–12, 2002. View at: Publisher Site  Google Scholar
 T.I. Wu and J.K. Wu, “The effects of chemical additives on the hydrogen uptake behavior of Ti6Al4V alloy,” Materials Chemistry and Physics, vol. 80, no. 1, pp. 150–156, 2003. View at: Publisher Site  Google Scholar
 H. H. Uhlig and R. W. Revie, Corrosion and Corrosion Control: An Introduction to Corrosion Science and Engineering, John Wiley & Sons, 1985.
 P. Marcus, Corrosion Mechanisms in Theory and Practice, CRC Press, 2011.
 B.S. Lee, Effects of cyclic hydrogenation and subsequent solution treatment on the mechanical properties of Ti153 alloy [M.S. thesis], Department of Materials Engineering, Tatung University, Taipei, Taiwan, 2012.
 J.C. Wu and T.I. Wu, “Influences of the cyclic electrolytic hydrogenation and subsequent solution treatment on the hydrogen absorption and evolution of βsolution treated Ti6Al4V alloy,” International Journal of Hydrogen Energy, vol. 33, no. 20, pp. 5651–5660, 2008. View at: Publisher Site  Google Scholar
 T.I. Wu and J.C. Wu, “Effects of cathodic charging and subsequent solution treating parameters on the hydrogen redistribution and surface hardening of Ti6Al4V alloy,” Journal of Alloys and Compounds, vol. 466, no. 12, pp. 153–159, 2008. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2013 ChienLung Huang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.